PHYSICAL REVIEW B VOLUME 58, NUMBER 18 1 NOVEMBER 1998-II Scaling of magnetization and some basic parameters of Ba12x Kx BiO31y superconductors near T c S. N. Barilo, S. V. Shiryaev, and V. I. Gatalskaya Institute of Physics of Solids and Semiconductors, Academy of Science, Minsk 220072, Belarus J. W. Lynn Center for Superconductivity Research, University of Maryland, College Park, Maryland 20742 and NIST Center for Neutron Research, National Institute of Standards and Technology, Gaithersburg, Maryland 20899 M. Baran, H. Szymczak, and R. Szymczak Institute of Physics, Polish Academy of Science, Warsaw PL 02-668, Poland D. Dew-Hughes Department of Engineering Science, Oxford University, Oxford OX1 3PJ, United Kingdom ~Received 10 June 1998! Reversible magnetization and hysteresis loops have been studied over wide ranges of magnetic field and temperature for single crystals of Ba12x Kx BiO31y (x50.34, 0.37, 0.41, and 0.46!. The main goals were to derive critical parameters of superconductors with a cubic structure as well as to explain the origin of flux pinning and peak ~fishtail! effect observed in all samples. Values of the electron-phonon interaction constant of l ph;1, ;0.76, and 0.9 for Ba12x Kx BiO31y with x50.34, x50.37, and x50.41, respectively, have been obtained. The data show that this family belongs to oxide superconductors with at least an intermediate strength of coupling. The pinning force density has been scaled into a single curve for wide field and temperature ranges. The functional form of the scaling curve reflects various mechanisms of flux pinning. For Ba0.54K0.46BiO31y the peak effect is mainly due to a dynamical contribution. However, the fishtail for Ba12x Kx BiO31y with x50.34, 0.37, and 0.41 has its origin in the crossover between two pinning mechanisms induced by external magnetic field and/or temperature. For the Ba0.59K0.41BiO31y crystal a seeded growthinduced anisotropy was found to be responsible for differences in low-field susceptibility and in hysteresis loops observed for different magnetic-field orientations. @S0163-1829~98!00442-1# I. INTRODUCTION Despite intense interest in such a promising compound like the isotropic superconductor Ba12x Kx BiOy ~BKBO! the question of the mechanism responsible for superconductivity at T c ;30 K and of the magnitude of the coupling constant remains open. Experimental studies to determine the energy gap value D 0 , the isotopic coefficient a, and the electronphonon interaction constant l ph are known to provide very important information for the solution of this problem. For conventional weak-coupling BCS superconductors the constant 2D 0 /k B T c has the value of 3.53,1 while for BKBO the value determined from a superconductor–insulator–normalmetal ~SIN! configuration of tunneling measurements2–7 ranges from 3.7 to 4.1 indicating intermediate to strong coupling. Experimentally determined critical parameters of BKBO superconductors obtained by different authors for single crystals, ceramics, and films are listed in Table I. As can be seen, the results of measurements of thin BKBO films in the high-frequency19 and IR Ref. 16 ranges agree well with the findings of tunneling measurements of D 0 and again indicate also the intermediate character of coupling in this compound. The early observation of the isotope effect in BKBO ~Ref. 10! yielded fairly conflicting results. The theoretical value of the isotopic coefficient a 5d ln Tc /d ln m in BCS superconductors is 21 ,27 assuming that neither Coulomb interaction nor 0163-1829/98/58~18!/12355~13!/$15.00 PRB 58 anharmonic optical modes are present. In Refs. 10, 28, and 29 a values were determined to be 0.20, 0.4, and 0.42, respectively, while in a recent paper23 an influence of potassium concentration on a in the Ba12x Kx BiO3 compounds has been found. The authors found that the isotopic coefficient a increases with the decreasing potassium concentration @a 50.21 (x50.45), 0.26 (x50.375), and 0.34 (x50.36)#, while the energy-gap values 2D 0 / k b T c vary from 4.0 (x 50.45) to 4.5 (x50.375), and 4.8 (x50.36). Accordingly, the coupling-constant estimations l ph are 1 (x50.45), 1.45 (x50.375), and 1.80 (x50.36), respectively,23 and indicate strong coupling. These results are connected with the conclusions30 about the growth of the coupling constant l ph as the potassium concentration approaches the superconductor-insulator boundary (x;0.35). From investigations of transport properties of BKBO crystals9 the coupling-constant value l ph51.7– 2.1 was determined, arguing that BKBO cannot be treated as a conventional weakly coupled superconductor. The value l ph52 has been obtained from dynamic susceptibility measurements on superconducting BKBO powder.26 However, in Ref. 14 the electron-phonon interaction parameter calculated from the magnetic and resistivity measurements of critical parameters of Ba0.62K0.38BiO3 single crystals was 0.48–0.96. From the examination of the structure phase diagram of Ba12x Kx BiO3 calculations of the constant of electron-phonon interaction for 0<x<0.5 were made20 and revealed a correlation of l ph 12 355 ©1998 The American Physical Society ;1b ~Ref. 3! 0.1b ~Ref. 17! 0.9a ~Refs. 20 and 21! 1.7–2.1b ~Ref. 9! 1–1.18b ~Ref. 23! 0.48; 0.96b ~Ref. 14! 2a ~Ref. 26! 1b ~Ref. 12! 3.5b ~Ref. 12! 3.5b ~Ref. 16! 3.8c ~Ref. 19! 3.7–4b,c ~Refs. 2–7! 4.1b ~Ref. 7! 4–4.8b ~Ref. 23! 2.4a,b ~Ref. 11! 1.5a ~Ref. 10! 0.3a ~Ref. 18! 3.4a ~Ref. 21! 2.36a ~Ref. 13! 2.31b ~Ref. 14! 50a,b ~Ref. 11! 59a ~Ref. 13! 21a ~Ref. 8! 60–68 ~Ref. 14! 51a,b ~Ref. 11! 46c ~Ref. 15! 36.8a ~Ref. 13! 32b ~Ref. 9! 45.3a ~Ref. 8! 39–45a ~Ref. 14! 24 p M ~ T,H ! 5 F f0 h H c2 ~ T ! ln 2 l H 8 p l L~ T ! G 16p k B l 2L ~ T ! 4 p k BT 2 ln , f 0 C j ~ T ! af 0 j 3 ~ T ! H Ae ~1! b Ceramics. Single crystals. c Thin and thick films. where the first term describes the London regime with the linear M (H) dependence,32 and the second part arises as a result of thermodynamic fluctuations,33 f 0 is the magnetic flux quantum, and h /l, a, C are constants of the order of unity that depends on the structure of the vortex lattice; j is the coherence length. It is recognized that thermodynamic fluctuations in high-T c cuprates can affect significantly the field dependence of magnetization and make a distinct contribution of the fluctuations into the M (H) behavior at high temperatures.34 The temperature range DT5GT c , where fluctuations effects are observable, is determined by the Ginzburg parameter G, estimated for BKBO crystals previously as ;331024 to be markedly lower than one for cuprates with the order of G51022 – 1023 . 35 So, the use of a shortened first term of Eq. ~1! in analyzing the BKBO magnetization data at temperatures near T c is quite justified. The constant h /l vanishes under differentiation of the first part of expression ~1! with respect to ] ln H: a ;0.5a,b ~Refs. 9 and 10! 0.57b ~Ref. 11! 0.78c ~Ref. 15! 0.52b ~Ref. 17! 0.87a ~Ref. 13! 0.78b ~Ref. 14! 0.9a ~Ref. 8! 32b ~Ref. 9! 16–21b ~Ref. 14! 15.4a ~Ref. 8! 17.3a ~Ref. 13! 12.6b ~Ref. 11! 15.2c ~Ref. 15! .25b ~Ref. 25! 8a ~Ref. 8! 35a ~Ref. 13! 100b ~Ref. 11! 95b ~Ref. 14! 400b ~Ref. 22! PRB 58 values with the experimental dependence of T c (x). 30 To illustrate, for potassium content x50.4, l ph50.95.20 Thus, we believe that BKBO can be considered as a conventional BCS superconductor with intermediate coupling. However, the coupling constant l ph50.35 determined in Ref. 17 also supports the assumption of weak coupling in this material, which runs counter to the findings given in Ref. 21, where l ph was estimated from the specific-heat measurements for the Ba12x Kx BiO3 ceramic sample to be of 0.9, and corresponds to intermediate coupling. The calculation31 of thermodynamic properties of Ba0.7K0.3BiO3 in terms of the Eliashberg theory on the assumption of an electron-phonon interaction gives the following values: 2D 0 /k B T c 54.15 and l ph51.18, i.e., this superconductor possesses strong coupling ~Table I and references cited therein!. The magnetic-field penetration depth l L is an exceptionally important characteristic of a superconductor and its temperature dependence l L (T) is very sensitive to the character of the coupling. In some papers concerned with measurements of the l L (T) by the muon-spin-rotation technique24 and resonant measurement in the high-frequency range,19 it was shown that BKBO is a weakly coupled BCS superconductor with l L (0)53300– 3400 Å. One way of determining the temperature dependence of l L (T) is measurement and analysis of reversible magnetization isotherms M (H) in the intermediate magnetic fields range H c1 <H<H c2 . In this region the following relationship between the magnetization and the magnetic field is valid for high-T c superconductors: 803a ~Ref. 8! 2200a ~Ref. 13! 2500b ~Ref. 11! 2700b ~Ref. 14! 3300c ~Ref. 19! 3400c ~Ref. 24! k 2dH c2 /dt ~T/K! lL ~Å! j ~Å! g (mJ/mol K2) S. N. BARILO et al. H c2 (0) ~T! H c1 (0) ~Oe! TABLE I. Critical parameters of Ba12x Kx BiO3 superconductors from different experiments. 2D 0 /kT l ph 12 356 ]M f0 5 . 2 2 ] ln H 32p l L ~ T ! ~2! Relation ~2! for accessible magnetic fields is usually applicable in a limited temperature range close to T c for an isotropic superconductor free of vortex-lattice pinning. One can determine the slope dM /ln H and hence the magnetic-field PRB 58 SCALING OF MAGNETIZATION AND SOME BASIC . . . penetration depth l L for various temperatures and analyze l L (T) in terms of the mechanism of pairing. In our previous paper36 a preliminary estimation of l L for BKBO single crystals has been given. In this work we have carried out systematic investigations of reversible magnetization M (H) isotherms near T c on the same single crystals with the aim of determining the temperature dependence l L (T), critical fields, and other Ginzburg-Landau parameters. The heatcapacity jump, corresponding to the superconducting transition of the BKBO crystal, and the constant of electronphonon interaction are also estimated ~Sec. III A!. Exploration of the temperature and field dependencies of the bulk pinning force density F p , defined as u J c B u , 37 is a particularly advantageous method for analysis of the pinning mechanism in superconductors. The pinning force scaling F p (b), where b5B/B c (B c 2 , the upper critical field!, is generally examined in conventional Nb3Sn superconductors, since the functional form F p (b) has frequently allowed conclusions to be drawn about the nature of pinning in the material. This asymptotic expression for the bulk pinning force has been first derived in Ref. 38 for niobium alloys: F p 5const3 @ B c 2 ~ T !# 2.5 f ~ b ! , ~3! where f (b) depends only on the normalized magnetic field. To put it differently, the knowledge of F p and f (b) for a hard superconductor at temperature T 1 permits one to obtain F p at any fixed temperature T 2 . In Ref. 37 the possibility of the flux-creep effect on the scaling F p has been dealt with to show that it can be ignored in the case of hard superconductors. Campbell and Evetts,39 as well as Dew-Hughes,40 have demonstrated that in conventional hard superconductors the pinning force density F p by and large can be represented as F p 5F p 0 ~ T ! b p ~ 12b ! q , ~4! where p,q depends on ~i! the defect dimensionality ~point, two-dimensional, or bulk!, ~ii! the type of interaction ~core pinning or magnetic pinning!, and ~iii! the nature of pinning center ~normal or superconducting!. According to Kramer’s theory, based on the vortex-lattice shear model, the pinning force follows expression ~4! while the coefficients p and q depend on the elastic properties of the vortex lattice and at large b value f (b);(12b) 2 . 41 The deviation from the scaling law for F p (4), in turn, with changing temperature and magnetic field can be related to the effects decaying the asymptotic behavior F p (b), for instance, the flux-creep effect and matching effect specified by commensurability of the vortex-lattice period and crystal microstructure, as well as of the various nature and size of pinning centers.39 A number of studies on the scaling F p in LaSrCuO,42,43 YBaCuO,44–52 BiSrCaCuO,51,53 and TlBaCuO ~Ref. 54! have been reported. A high-temperature superconductor ~HTSC! is distinguished from a conventional hard superconductor by high values of T c , short coherence length, large spatial anisotropy, and lower activation energy of pinning. This also influences the pinning force scaling law F p as the critical current and bulk pinning force decrease to zero with the irreversibility field B irr which is much lower than B c 1 . A set of fields B irr(T) constitutes scaling fields for HTSC materials, and the scaling law for the bulk pinning force is 12 357 F p ~ b 8 ,T ! 5F p 0 ~ T ! f ~ b 8 ! 5F p 0 ~ T ! b 8 p ~ 12b 8 ! q , ~5! where b 8 5B/B irr(T). In the majority of HTSC materials over a broad range of external fields the above-mentioned scaling F p has been observed. However, the exponential fall of magnetization with increasing magnetic field is frequently seen at large fields, i.e., the term 12b 8 in Eq. ~5! on this section of the phase diagram B-T should be replaced by b exp(2b/b8). In this connection, the conclusion has been drawn that one should not expect a perfect scaling F p for high-T c superconductors in so far as the effect of the flux creep and flux flow cannot be neglected.55 At elevated temperatures, F p (B,T) is determined not only by the critical current density in the absence of activation process J c 0 5F p 0 /B, but also by the activation energy u( g ,B,T). Alternatively, in the low-temperature range the flux creep is insignificant. In some HTSC compounds, for instance in the overdoped LaSrCuO,50 F p does not obey Kramer’s scaling law.42 The pinning force density scaling law of the Ba12x Kx BiO31y ~BKBO! superconductor with T c '30 K, which are intermediate between conventional and layered high-T c superconductors, is not understood yet. These compounds feature a simple-cubic structure, along with the absence of CuO2 phases and magnetic ions in the lattice. We have first seen and studied comprehensively the peak effect in magnetization for BKBO single crystals with x>0.33.36 The peak F p max(H) shifts to the upper-field range with the temperature decreasing while its value rises. The value of the normalized pinning force F p /F p max 5f(H/Hmax) is scaled to a single curve up to H max for all the measured isotherms. However, the scaling was disrupted at higher fields. In this paper we report on a comprehensive study of the field dependence of the bulk pinning force F p for BKBO single crystals with various potassium concentration, and of the scaling law in dependence of temperature aimed at interpreting the peak effect nature in high-T c superconductors with isotropic structure ~Sec. III B!. We have also investigated the effect of seeded growth-induced anisotropy on magnetic properties of BKBO (x50.41) single crystal in superconducting state ~Sec. III C!. II. SAMPLES AND EXPERIMENTAL TECHNIQUE Magnetic measurements were taken from four single crystals of BKBO. The electrodeposition growth method was used for all the samples. The first three crystals, with potassium concentration x50.34, 0.37, and 0.46, respectively, and typical dimensions of 23232 mm3, were grown by spontaneous crystallization56 and exhibited T c 519.5– 31 K depending on the potassium concentration. The fourth one, with x50.41, was prepared by the seeded growth technique that allows fairly large crystals up to 2 cm3 to be grown with T c ;31 K and a relatively narrow superconducting transition to be obtained. The fourth sample had approximately cubic shape with dimensions 1.9231.9031.90 mm3 and was cut from a central part of as-grown large crystal (10315 35 mm3). All faces of the sample are oriented ~100!-type planes. One of them is the natural growth surface. To reveal any effects related to the growth-induced anisotropy the chemical etching technique has been applied to neighboring 12 358 S. N. BARILO et al. PRB 58 FIG. 1. The stripe defects structure oriented parallel to the natural ~001! growth surface of Ba0.59K0.41BiO31y single crystal was revealed by chemical etching on perpendicular cut of the sample ~none could be found on the cut parallel to natural face!. parts of the same crystal. As a result, a stripe structure parallel to the growth surface on faces cut perpendicular to this one was found. No such structure was obtained on faces parallel to the growth surface. The period of etched defects structure was 1–2 mm ~Fig. 1!. The first indication in microstructure evidence to indicate what might be responsible for the pinning is presented below. As has been mentioned, the sample with x50.41 reveals the seeded growth-induced anisotropy. Small-angle neutron scattering ~SANS! was employed to investigate this structure, and the SANS pattern obtained at room temperature is shown in Fig. 2. The experiments were carried out on the NG-7 spectrometer at the NIST Center for Neutron Research, using both moderate and high resolution. These data were taken with a neutron wavelength of 12 Å, no guides, and the two-dimensional positionsensitive detector at a distance of 12 m from the sample. The square-shaped pattern has its corners in the @110# crystallographic direction, and the intensity in any particular direction falls off as 1/Q 4 . This Porod-type scattering indicates that the structural defects producing the scattering are considerably larger than the range explored here, consistent with the optical micrographs that suggest a length scale of ;1 mm. The potassium concentration of all measured samples was determined by three methods: ~1! from x-ray measurements of the crystal-lattice parameters according to the calibration curve;30 ~2! from neutron activation analysis; ~3! from the measurements of natural radioactivity of the isotope 40K. The reversible ~irreversible! magnetization and susceptibility on the BKBO single crystals at low fields in fieldcooled and zero-field-cooled conditions were recorded with a superconducting quantum interference device magnetometer FIG. 2. The SANS patterns at two different orientations of Ba0.59K0.41BiO31y single crystal in the ~001! face: ~a! x axis of the picture coincides @100# crystal direction; ~b! x axis of the picture lies alone @110# crystal direction. FIG. 3. Isotherms of magnetization vs the logarithm of the applied field for Ba0.59K0.41BiO31y single crystal ~open and solid symbols denote data measured at increasing and decreasing applied field, respectively!. ~Quantum Design, MPMS-5! over a range of temperature 3–40 K and magnetic fields up to 50 kOe. The susceptibility of crystals in the normal state was determined over the temperature range from 40 to 300 K in the field of 6 and 50 kOe and thereafter this contribution was subtracted from the M (H,T) dependencies to pick out the magnetic response related to the superconducting state of the crystal. III. RESULTS AND DISCUSSIONS An analysis of hysteresis loops M (H) for the BKBO single crystals with various potassium concentration show that all the measured crystals featured the peak effect on magnetization curves over a definite temperature range. The position of extra maximum on the hysteresis loops is temperature dependent, and the field of the peak effect H p decreases with increasing temperature. The measurements in the high field and temperature range exhibit M (ln H) dependencies that are straight lines and are successfully described by relation ~1! in the field and temperature regions under investigation. A. Reversible magnetization range Figure 3 shows measured isotherms M (ln H) of BKBO for the x50.41 crystal, which are typical for all the crystals. PRB 58 SCALING OF MAGNETIZATION AND SOME BASIC . . . 12 359 TABLE II. Critical fields and Ginzburg-Landau parameters of Ba12x Kx BiOy single crystals obtained from magnetization measurements. Composition of the single crystal Critical parameter of superconductor Ba0.66K0.34BiO3 Ba0.63K0.37BiO3 Ba0.59K0.41BiO3 T c @K ~low field!# H c2 ~0! ~T! dH c2 /dT ~T/K! j~0! ~Å! l L ~0! ~Å! k~0! H c1 (0) ~Oe! H c ~0! ~T! DC/T c , (mJ/mole K2) g mJ/mole K2 N(E F ) ~states/eV cell! l ph 30 25.0 20.78 36.4 ;3089 ;85 77 0.21 3.1 2.16 ;0.46 ;1 29 19.3 20.65 41.5 ;3100 ;75 74 0.18 2.57 1.8 ;0.40 ;0.76 31 20.9 ;0.6 40 3200 80 73 0.187 2.79 1.95 0.44 ;0.9 The experimental data are well described by the logarithmic field dependencies in the investigated temperature range. From the same data, using relation ~2!, we obtained the temperature dependencies of the magnetic-field penetration depth l L represented in Fig. 4. Curves l L (T) are well described by the classical BCS formula l L (T)5l L (0)(1 2t) n , where t5T/T c , T c is the superconducting transition temperature, and an exponent of n;0.5. The values l L (0) as well as some other experimental and calculated parameters of superconducting single crystals are listed in Table II. As can be seen, the experimentally determined values of penetration depth l L (0) for BKBO known in the literature vary from 803 to 3300 Å.19,26,14,8,13,11,22 It must be emphasized that normal inclusions that may be present in the sample can lead to underestimating the magnetization value. Since l 22 L is proportional to the ] M / ] ln H, the value of penetration depth l L can be overestimated by a constant multiplier, though the character of the temperature dependence of l L (T) remains the same. But we should mention also that x-ray and neutron analysis of our crystals57 exhibited single-phase character and a high degree of perfection of the as-grown crystals as well as practically no normal inclusions. The value of magnetic susceptibility of the crystals in the normal state, which in the high-temperature range is consistent with the data given by other authors,10,21 verifies the single-phase structure. For this reason we have not recalculated the values of penetration depth related to the possible presence of normal ranges in crystals. Our recent paper,36 which deals with estimation of the temperature dependence of the upper critical magnetic field H c2 (T) for our single crystals, reveals that near T c , H c2 (T) is well described by the linear relation that correlates with the Ginzburg-Landau theory. The values of H c2 (0) and ( ] H c2 / ] T) T c are listed in Table II with the data. The coherence length j~0! calculated from the relation H c2 5 f 0 /2pj 2 equals 36.4 Å (x50.34), 41.5 Å (x50.37), and 40 Å (x50.41). With the values for l L (0), we can evaluate the Ginzburg-Landau parameter values to be k 5l L / j ;85 (x50.34), ;75 (x50.37), and 80 (x50.41), respectively. We may then estimate the specific-heat jump at T c in accordance with relation58 DC/T c 5 F G ] H c2 2 1 . 2 8 p gk ]T ~6! The Sommerfeld constant g has been calculated through the use of the relation DC/T c 51.43g ~Table II!. As can be seen, the g values are close to the corresponding data obtained for melted Ba0.65K0.35BiO3 ( g 52.36 mJ/mol K2), 8 for Ba0.6K0.4BiO3 ( g 53.4 mJ/mol K2) ceramic sample,18 and FIG. 4. Temperature dependence of the magnetic-field penetration depth for Ba0.59K0.41BiO31y single crystal, derived on the basis of relation ~2!, which agrees well with the BCS formula @solid line, l 0 ~the penetration depth value at zero temperature!#. Inset: the same dependencies for Ba0.66K0.34BiO31y and Ba0.63K0.37BiO31y single crystals. S. N. BARILO et al. 12 360 PRB 58 FIG. 5. The isotherms of normalized pinning force F p /F p max as a function of the reduced field b5H/H irr for the Ba0.66K0.34BiO31y single crystal. It can be seen that experimental values of reduced pinning force are satisfactorily approximated by two different 8 of 0.56 @2D curves having a peak, according to relation ~5!, for b max pinning on Dk centers ~dotted line!# and 0.22 @2D pinning on normal centers ~dashed line!#. Ba0.62K0.38BiO3 ( g 52.31 mJ/mol K2) single crystal.14 From the value of g one can determine the resulting electron density of states at the Fermi level N * (E f ) in accordance with the expression g 52/3p 2 k 2B N * ~ E f ! . ~7! The electron-phonon interaction constant l ph can also be determined from N * (E f )5N(0)(11l), where N(0) is the electron density of states of order 0.23 states/eV cell as follows from the band-structure calculations for BKBO ~Ref. 59! ~see Table II!. The values of l ph;1, ;0.76, and 0.9 point to the fact that the single crystals Ba12x Kx BiOy with x50.34, x50.37, and x50.41, respectively, are superconductors with intermediate coupling. From analysis of the magnetic susceptibility data for the BKBO single crystals in the normal state there was obtained at temperatures from 250 to 300 K the value x is 25 31025 emu/mol (x50.34) and 2431025 emu/mol (x 50.37). In general, the magnetic susceptibility of the crystal in the normal state x consists of several contributions60 connected with ~1! the Pauli paramagnetism x P ; ~2! the Landau diamagnetism of conduction electrons x L ; ~3! the Van Vleck paramagnetism x VV ; ~4! the electron core diamagnetism x core ; and ~5! paramagnetism of impurities x imp . The last contribution for BKBO crystals is very small. This is also consistent with insignificant volume of normal areas as assumed by us in the investigated crystals. The value of x L 52(m/m * ) 2 x p /3 and, assuming that m * /m;7 – 8 ~Ref. 21! FIG. 6. ~a! and ~b! The isotherms of the normalized pinning force F p /F p max as a function of the reduced field b5H/H irr for Ba0.63K0.37BiO31y single crystal fitted to Eq. ~5! @fittings reveals 8 of 0.12 ~dotted line! and 0.6 ~dashed line!; solid line correb max sponds to the sum#. As can be clearly seen, the character of vortex pinning changes drastically in 23<T<24 K due to a type of 2D pinning-center variation. for BKBO (x50.4), the diamagnetic contribution of conduction electrons x L constitutes a negligibly small fraction of x P . The contribution of x VV is also disregarded by us and the magnetic susceptibility of the BKBO single crystals becomes x 5 x P 1 x core . The last value can be estimated from the tabulated values of the radii of occupied electron shells for Ba21, K11, Bi31, and O22: 61 x core527.8 31025 emu/mol. On this basis we derive the values 2.67 31025 emu/mol (x50.34) and 3.731025 emu/mol (x 50.37) for a contribution of the Pauli paramagnetism. The PRB 58 SCALING OF MAGNETIZATION AND SOME BASIC . . . 12 361 TABLE III. List of F p scaling low parameters for Ba12x Kx BiO31y single crystals with different potassium content. Sample no. 1 2 3 4 5 Potassium content x n 0.34 0.59 0.37 Exponent value m p 0.77 q Exponents 8 ratio b max Temperature ~K! 1.95 1.52 0.56 19–22 0.48 4.60 1.70 3.10 0.22 0.60 24–28 20–22 0.43 0.853 3.20 8.82 0.12 0.09 25–27 1.21 2.93 0.78 6.39 9.8 0.31 0.07 1.21 1.18 2.96 0.58 6.58 2.94 0.31 0.16 1.45 1.22 0.41 (H'surface) 19–27 0.41 (H i surface) 0.46 19–27 1.40 resulting density of electron states at the Fermi level is related to the Pauli susceptibility through the well-known expression x p 5N A ~ 2 m 2B ! N * ~ E f ! 5230.323331024 N * ~ E f ! , ~8! where N A is Avogadro’s number and m B is the Bohr magneton. The value of the density of states N * (E f ) determined from the Pauli susceptibility in accordance with Eq. ~6! is 0.42 and 0.56 states/eV cell for crystals with x50.34 and x 50.37, respectively. Hence, the total sum of the density of states N * (E f ) calculated in terms of the specific-heat jump close to T c ~Table II! and of magnetic susceptibility in the normal state agree satisfactorily. Earlier we have estimated by SIN tunneling measurements the superconducting gap magnitude of 2D 0 /k B T ;4.1,7 which is significantly larger than the value of 3.5 for an ideal weak-linked BCS superconductor. In accordance with the Toxen empirical formula the gap and thermodynamic critical field H c are related at low temperature by62 2D 0 /k B T c 52T c /H c0 „] H c ~ T ! / ] T…, 12–18 H irr(T);(12T/T c ) m , though mÞn. The exponents n and m vary depending on potassium content in the crystal as listed in Table III. The analysis of the field-dependent value DM H (DM is a hysteresis loop width and H;B), proportional to the pinning force density, has revealed a similar pattern in the temperature range T<20 K for all the investigated crystals. The F p (H) function goes through a maximum and shifts to a lower field range as the temperature increases, while the maximum amplitude decreases. The normalized pinning force values F p /F p max5f(b!), where b ! 5H/H max for all the ~9! where D 0 and H c0 are the gap and thermodynamic critical field values at T50. Note that two independent crystal characteristics, the gap and the slope of H c (T) at T c are combined by relation ~9!. The right part of Eq. ~9! was calculated from magnetization data to be of 4.0. The small ~;2.5%! difference between SIN tunneling and calculated data allows us to determine that BKBO is not a weak-link superconductor. The relation E v 5H 2c H c1 /2H c2 also provides an estimate of the energy of vortex nucleation of E v /(H 2c /8p ) ;4.7531023 . B. Irreversible magnetization range As was mentioned above, all the crystals that have been measured reveal the peak effect in magnetization curves over a broad temperature range. The temperature dependence of H p is described well by the power law H p ;(12T/T c ) n . The irreversibility line H irr(T) is also described by the function FIG. 7. The isotherms of normalized pinning force F p /F p max as a function of the reduced field b5H/H irr for the Ba0.54K0.46BiO31y single crystal scaled to a single curve by the unified pinning mechanism over the whole temperature range investigated ~fitting reveals 8 of 0.16 corresponding to single vortex pinning by randomly b max distributed 2D normal centers!. 12 362 S. N. BARILO et al. FIG. 8. The isotherms of normalized pinning force F p /F p max as a function of the reduced field b5H/H irr for Ba0.59K0.41BiO31y single crystal scaled to Eq. ~10!: ~a! H' the natural crystal surface @p50.85, q58.82 ~dotted line!; p 8 52.93, q 8 56.39 ~dashed line!#; ~b! H i the growth surface of crystal @p50.78, q59.8 ~dotted line!; p 8 52.96, q 8 56.58 ~dashed line!#. The data seem to indicate, similarly as for Ba0.54K0.46BiO31y , the importance of the d1 pinning related to the spatial variation of the charge-carrier mean free path. crystals are aligned with one curve up to H max ~see, for example, Ref. 36!. For temperatures T.23 K near T c , though, the deviation from the single asymptotic behavior in the whole magnetic field range is clearly seen. For instance, compounds with x50.34, 0.37 tend to change the character of dependence as the temperature rises from a curve with a narrow peak to a curve with a broader one. The normalized pinning force density of the investigated BKBO crystals yielded via expression ~5! the scaling param- PRB 58 FIG. 9. Temperature dependencies of ~a! the magnetic shielding ~zero-field cooled! and ~b! the Meissner ~field cooled! signals for the Ba0.59K0.41BiO31y single crystal ~with demagnetizing factor taken in account!. Field-cooled Meissner susceptibility is distinctly different for both field orientations in the whole temperature range indicating a stronger pinning in low fields for H' . eters that are listed in Table III. Examples of fitted curves are presented in Figs. 5–8. It is well known that p,q for conventional hard superconductors, as well as for coppercontaining HTSC YBa2Cu3O72d ~YBCO!,43,51 BiSrCaCuO,52 and TlBaCuO.53 In our case this condition is satisfied with the BKBO single crystals of potassium content x50.41 (T 519– 27 K), x50.46 (T512– 18 K), but for x50.34 and 0.37 at temperatures close to T c only. The condition p,q is in agreement with the concept of the critical shear strength of the flux lattice introduced by Kramer.41 However, in the lower temperature range the relation p.q was obtained for PRB 58 SCALING OF MAGNETIZATION AND SOME BASIC . . . crystals with x50.34 and 0.37 ~Figs. 5 and 6!. As could be clearly seen in Figs. 6~a! and 6~b!, the character of vortex pinning changes drastically at T<23 K for the sample with x50.37. It is recognized40 that the peak positions on F p /F p max 5f(b8) curves point out to the pinning mechanism and could be determined as b 8max5p/(p1q). The b 8max values for crystals with different composition are also summarized in Table III. From Figs. 5 and 6, in accordance with the above-mentioned model, one can make an assumption for crystals with x 50.34 and 0.37 about ~i! the character of the pinning centers being two dimensional ~2D!; ~ii! two different types of pinning centers ~normal and Dk!; ~iii! the peak effect being due to the crossover between at least two different pinning mechanisms induced by external magnetic field and/or temperature. For the BKBO single crystals with x.0.33, as established in Ref. 36, the peak effect exists though no exhaustive explanation has been provided. In the YBCO and BiSrCaCuO systems the peak effect occurs but has a different interpretation. Thus in the case of YBCO the peak effect is accounted for by employing ~i! the model of superconductivity depression by a magnetic field in oxygen-deficient ranges that become the pinning centers63 or ~ii! the model of crossover from the single to collective flux creep leading to the reduction of magnetization relaxation in intermediate fields.64 The matching effect has been proposed in Ref. 65 to explain the peak effect in BiSrCaCuO. The peak effect in Tl-based single crystals is related to the softening of the vortex lattice making for the pinning efficiency with plausible 3D to 2D transition or melting of the 3D lattice; in this instance the anisotropy of electronic properties g 5(m !c /m !ab ) 1/2 is favored. The findings for scaling law for the bulk pinning force in cubic single crystals of BKBO with various potassium concentration indicate that the peak effect in crystals with x 50.34 and 0.37 is related to the crossover of two pinning mechanisms as the magnetic field increases. At the same time our observation of the scaling behavior of the crystal with x50.46 ~Fig. 7! is well described by the unified pinning mechanism over the whole temperature range investigated. From our earlier study on the same sample, the dependence of the relaxation rate value of S(H) at different temperatures has been plotted. The S(H) peaks on the isotherms were observed for H;0.5H p (H p marks the peak-effect field!.36 These data contradict the suggestion that dimensional crossover between 3D and 2D vortex stricture causes the peak effect in the sample. The detailed analysis with the prediction of the theoretical models describing so-called d T c and d1 pinning65 revealed a conclusion that the single-vortex pinning by randomly distributed 2D normal centers occurs in the crystal with x50.46. C. Seeded growth-induced anisotropy and pinning centers for Ba0.59K0.41BiO31y The first indication in microstructure evidence to indicate what might be responsible for the pinning is presented below. As have been mentioned, the sample with x50.41 reveals the seeded growth-induced anisotropy. The stripe 12 363 FIG. 10. Volume magnetization hysteresis loops for two different orientations of the field to the natural growth surface of Ba0.59K0.41BiO31y single crystal. Inset: for better presentation of peak effect, the low-field region is omitted. structure of defects oriented parallel to the natural growth surface of crystal has a period approximately of 1 mm ~Fig. 1!. The critical temperature T c as obtained from the extrapolation of the maximum slope of x (T) to x 0 , determined from x (T) after zero-field cooling in an applied field of 10 Oe, is equal to 30.5 K ~Fig. 9!. This value is greater than those observed previously for BKBO (x50.34, 0.37, and 0.46! crystals.35 Such a value of T c indicates that the oxygen concentration is close to the optimal one @y'20.05 ~Ref. 66!#. The shielding effect in H ext510 Oe is close to ideal of 1/4p taking into account a demagnetizing factor. The anisotropy in the zero-field-cooled data is reflected only in some differences in the transition region @Fig. 9~a!#. The fieldcooled Meissner susceptibility is distinctly different for both field orientations in the whole temperature range @Fig. 9~b!#, indicating stronger pinning in low fields in the case of the external field oriented perpendicular to the natural growth surface of crystal (H' ). On hysteresis loops a relatively weak peak effect was observed in the low-temperature range of 3–7 K. The position of the peak depends on the field orientation ~Fig. 10! being shifted to higher fields for H' . The width of hysteresis loop DM behaves as follows: ~a! the ratio of DM (H' )/DM (H i ) is a function of temperature and magnetic field, but its maximal value ~1.9–2.3! is practically independent of temperature in the range of 3–27 K. The position of this maximum shifts from higher to lower fields with increasing temperature. It changes from a broad maximum ~in the range from 25 up to 48 kOe! at low T ~3–7 K! to a somewhat complicated structure in small fields up to 1.5 kOe at 27 K @Figs. 11~a!, 11~b!, and 11~c!#; ~b! at temperature of T53 – 18 K, in the entire field range H<50 kOe the 12 364 S. N. BARILO et al. PRB 58 FIG. 11. ~a!, ~b!, and ~c! Ratio DM (H' )/DM (H i ) as a function of external magnetic field for several temperatures. It should be underscored that the condition DM (H' )/DM (H i ).1 is fulfilled except in the higher-field region at T>20 K in the rest of the H-T range investigated. value of DM (H' )/DM (H i ) is larger than 1; ~c! at 20 K and H>14 kOe the ratio is close to 1; ~d! at higher temperatures (T.20 K) and magnetic fields (14 kOe<H<H irr) the ratio is less than 1 ~reaching a minimum of about 0.6!. The irreversible magnetization anisotropy is clearly seen to be the opposite character of DM (H) curves cross sections under small and high external fields ~Fig. 12!. It should be emphasized that the condition DM (H' )/DM (H i ).1 is fulfilled except in the higher-field region, at T>20 K. This could be explained by taking into account the chemical etching experiments. The results could be understood assuming that during the seeded growth of crystal some kind of macroscopic layered structure was formed ~with a period of 1–2 mm, or even smaller, not detected by chemical etching technique we used!, which is responsible for an anisotropy of critical current. The interlayer borders play two different roles in the case of magnetic field oriented parallel to the natural surface (H i ): first of all, they act as weak links limiting the critical current density and second they act as twodimensional pinning centers. Weak links are responsible for the ratio DM (H' )/DM (H i ).1 in the majority of H-T space, whereas an existence of natural 2D pinning centers plays a significant role in the higher-field region at T >20 K resulting in DM (H' )/DM (H i ),1. Because the effectiveness of both mechanisms depends differently on temperature and magnetic field, this leads to a complicated dependence of the ratio versus H and T ~Fig. 11!. Simultaneously, some part of oxygen defects can be ordered along the direction normal to the natural surface as an effect of the application of an electric field of this direction PRB 58 SCALING OF MAGNETIZATION AND SOME BASIC . . . FIG. 12. The irreversible magnetization anisotropy for different external-field orientations to the natural surface for the Ba0.59K0.41BiO31y single crystal grown on a seed. Inset: the opposite character is clearly seen for DM (H) curves cross section under small and high external fields. during the crystal growth process. The presence of such rather low dimensional defects, which can be effective as pinning centers in low magnetic field of orientation H' , could be responsible for the difference in field-cooled susceptibility @Fig. 9~b!#. It has been found that the changes of the pinning force ~or rather its main contribution! with external magnetic field and temperature can be well described by the universal scaling law F p /F p max5Ab p1 ~ 12b ! q1 1Bb p2 ~ 12b ! q2 , ~10! where b5H/H irr @Figs. 8~a! and 8~b!#. The obtained results ~Table III! seem to indicate, similarly as for BKBO (x 50.46), the importance of the depinning related to the spatial variation of charge-carrier mean free path. The observed peak effect seems to be caused by a variation of the dl-pinning character due to a sharp change of pinning center geometry from a surface to a point with decreasing temperature. It was found that in the limit of the estimation of errors H irr does not depend on the field orientation. In the temperature range of 18–27 K, where the irreversibility field could be estimated, H irr displays a power law of the reduced temperature (T/T c ) according to the relation H irr5132(1 2T/30.5) 1.21 kOe. The reversible part of magnetization curves is identical for both applied-field orientations, which indicates the isotropy of penetration depth under these temperatures. IV. CONCLUSIONS We analyzed the reversible and irreversible magnetization near T c for Ba12x Kx BiO31y single crystals with different 12 365 potassium content. The isotherms of reversible magnetization were used to estimate the most important characteristics of the superconductors with a cubic structure. The values of the electron-phonon interaction constant of l ph;1, ;0.76, and 0.9 for Ba12x Kx BiO31y with x50.34, x50.37, and x 50.41, respectively, have been obtained. The data show that the family belongs to oxide superconductors with at least intermediate strength of coupling. It could be concluded now, from the irreversible magnetization data analysis, that pinning in cubic BKBO is caused by an interaction between either the flux-line lattice or individual vortices and the microstructure of the superconductor. The microstructure provides some spatial variation of the basic superconducting properties, and thus the strength of the pinning is related to the basic superconductivity, and therefore involves the thermodynamic critical field. For true pinning the scaling must be to the thermodynamic critical field, which, in turn, can, via k, be related to the upper critical field H c2 . If the pinning force is defined by the moment at which the flux breaks away from the pinning centers, then the scaling for the oxide superconductor will follow relation ~5!. If the flux lattice begins to shear, whether by the dislocation mechanism Dew-Hughes proposed,40 or by some other means, the critical Lorentz force is related to the properties of the flux-line lattice, and in particular, the elastic constants of the lattice. These usually show something that approximates F p ;b 1/2(12b) 2 and it is not unreasonable that in HTSO they might scale to the irreversibility field, i.e., b 5B/B irr , as this is the field at which the lattice constants go to zero. If we now look at our results, those for x50.46 ~Fig. 7! clearly indicate that at all temperatures the flux is so strongly pinned ~by the unified pinning mechanism over the whole temperature range investigated! that the lattice shears before unpinning. This is also the case for the other three compositions at temperatures near T c . The curves at the lower temperatures could scale as those that drive relation ~5! if the reduced field were related to B c2 rather than the lower B irr , with a cutoff as B irr is approached. This requires a mechanism whereby the flux is pinned at lower temperatures with a pinning strength less than the shear strength of the lattice, but which changes with temperature less sharply than does the lattice shear strength so that at high temperatures the lattice shears before it unpins. We can assume that such changes take place in BKBO (x50.41) with a high probability. In particular, the observed peak effect seems to be caused by a variation of the dl pinning character due to sharp change of pinning centers geometry from 2D to a point with decreasing temperature. From the data obtained we can conclude for crystals with x50.34 and 0.37 that ~i! there is 2D geometry of the pinning centers in all the temperature range observed; ~ii! there are two different types of pinning centers ~normal and Dk!; ~iii! the peak effect is due to the crossover between dl and d T c pinning mechanisms induced by external magnetic field and/or temperature. ACKNOWLEDGMENTS The work in Minsk and Maryland was supported in part by the CRDF program, Grant No. BP 1-111 and in Warsaw by the Polish State Committee for Scientific Research under Contract No. 2P30211407. 12 366 1 S. N. BARILO et al. J. Bardeen, L. N. Cooper, and J. R. Schiffer, Phys. Rev. 106, 162 ~1957!. 2 Q. Huang, J. F. Zasadzinski, N. Tralshawala, K. E. Gray, D. G. Hinks, J. L. Peng, and R. L. Greene, Nature ~London! 347, 369 ~1990!. 3 H. Sato, H. Takagi, and S. S. Uchida, Physica C 169, 391 ~1990!. 4 B. M. Moon, C. E. Platt, R. A. Schweinfurth, and D. J. Van Harlingen, Appl. Phys. Lett. 59, 1905 ~1991!. 5 J. F. Zasadzinski, N. Tralshawala, D. G. Hinks, B. Dabrowski, A. N. Mitchell, and D. R. Richards, Physica C 158, 519 ~1989!. 6 F. Sharifi, A. Pargellis, R. C. Dynes, B. Miller, E. S. Hellman, J. Rosamilia, and E. H. Hartford, Phys. Rev. B 44, 12 521 ~1991!. 7 P. Samuely, N. L. Bobrov, A. G. M. Jansen, P. Wyder, S. N. Barilo, and S. V. Shiryaev, Phys. Rev. B 48, 13 904 ~1993!. 8 H. C. Jang, M. H. Hsieh, D. S. Lee, and H. E. Horng, Phys. Rev. B 42, 2551 ~1990!. 9 M. Affronte, J. Marcus, C. Escribe Filippini, A. Sulpice, H. Rakoto, J. M. Broto, J. C. Ousset, S. Askenazy, and A. G. M. Jansen, Phys. Rev. B 49, 3502 ~1994!. 10 B. Batlogg, R. J. Cava, L. W. Rupp, A. M. Mujsce, J. J. Krajewski, J. P. Remeika, W. F. Peck, A. S. Cooper, and G. P. Espinosa, Phys. Rev. Lett. 61, 1670 ~1988!. 11 Z. I. Huang, H. H. Fang, Y. Y. Hue, P. H. Hor, C. W. Chu, M. L. Norton, and H. Y. Tang, Physica C 180, 331 ~1991!. 12 V. F. Gantmakher, L. A. Klinkova, N. V. Barkowskii, G. E. Tsadynzhapov, S. Wieger, and A. K. Geim, Phys. Rev. B 54, 6133 ~1996!. 13 W. K. Kwok, U. Welp, G. Crabtree, K. G. Vandervoort, R. Hulsher, Y. Zheng, B. Dabrowski, and L. G. Hinks, Phys. Rev. B 40, 9400 ~1989!. 14 T. Uchida, S. Nakamura, N. Suzuki, Y. Nagata, W. D. Mosley, M. D. Lan, P. Klavins, and R. N. Shelton, Physica C 215, 350 ~1993!. 15 R. A. Schweinfurth, C. E. Platt, M. R. Teepl, and D. J. van Harlingen, Appl. Phys. Lett. 61, 480 ~1992!. 16 Z. Schlesinger, R. T. Collins, J. A. Calise, D. G. Hinks, A. W. Mitchell, Y. Zheng, B. Dabrowski, N. E. Bickers, and D. J. Scalapino, Phys. Rev. B 40, 6862 ~1989!. 17 J. E. Graebner, L. F. Schneemeyer, and J. K. Thomas, Phys. Rev. B 39, 9682 ~1989!. 18 S. E. Stupp, M. E. Reeves, D. M. Ginsberg, D. G. Hinks, B. Dabrowski, and K. G. Vanderviirt, Phys. Rev. B 40, 10 878 ~1989!. 19 M. S. Pambianchi, S. N. Anlage, E. S. Hellman, E. H. Hartford, M. Bruns, and S. Y. Lee, Appl. Phys. Lett. 64, 244 ~1994!. 20 A. I. Liechtenstein, I. I. Mazin, C. O. Rodriguez, O. Jepsen, O. K. Andersen, and M. Methfessel, Phys. Rev. B 44, 5388 ~1991!. 21 G. K. Panova, A. A. Schikov, B. I. Savel’ev, A. P. Zhernov, N. V. Anschukova, A. I. Golovaschkin, A. I. Ivanova, and A. P. Rusakov, Zh. Éksp. Teor. Fiz. 103, 605 ~1993! @JETP 75, 478 ~1993!#. 22 S. N. Barilo, V. I. Gatalskaya, D. I. Zhigunov, L. A. Kurochkin, and S. V. Shiryaev, Supercond., Phys. Chem. Technol. 7, 753 ~1994!. 23 G. Zhao and D. E. Morris, Phys. Rev. B 51, 12 848 ~1995!. 24 T. J. Ansaldo, Z. R. Wang, J. H. Cho, D. C. Johnston, and T. M. Riseman, Physica C 185–189, 1889 ~1991!. 25 M. Kosuji, Z. Akimitsu, T. Uchida, M. Furuja, J. Nagata, and T. Ekino, Physica C 229, 389 ~1994!. 26 V. F. Gantmaker, L. A. Klinkova, A. M. Neminskii, and M. V. PRB 58 Filatova, Zh. Éksp. Teor. Fiz. 101, 1612 ~1992! @Sov. Phys. JETP 74, 859 ~1992!#. 27 J. P. Carbotte, Rev. Mod. Phys. 62, 1027 ~1990!. 28 D. G. Hinks, D. R. Richards, B. Dabrowski, D. T. Marx, and A. N. Mitchell, Physica C 162–164, 1405 ~1989!. 29 C. R. Loong, Phys. Rev. Lett. 66, 3217 ~1991!. 30 Sh. Pei, J. D. Jorgensen, B. Dabrowski, D. G. Hinks, D. R. Richards, A. W. Mitchell, J. M. Newsam, S. K. Sinha, D. Vaknin, and A. J. Jacobson, Phys. Rev. B 41, 4126 ~1990!. 31 O. Navarro, Physica C 265, 73 ~1996!. 32 V. S. Kogan, M. M. Fang, and S. Mitra, Phys. Rev. B 38, 11 958 ~1988!. 33 S. Mitra, J. H. Cho, W. C. Lee, D. C. Johnston, and V. G. Kogan, Phys. Rev. B 40, 2674 ~1989!. 34 V. G. Kogan, M. Ledvij, A. Yu. Simonov, J. H. Cho, and D. C. Jonston, Phys. Rev. Lett. 70, 1870 ~1993!. 35 G. Blatter, M. V. Feigelman, V. B. Geshkenbein, A. I. Larkin, and V. M. Vinokur, Rev. Mod. Phys. 66, 1125 ~1994!. 36 H. Szymczak, M. Baran, R. Szymczak, S. N. Barilo, V. I. Gatalskaya, and S. V. Shiryaev, SPIE Proc. 3178, 262 ~1997!; S. N. Barilo, V. I. Gatalskaya, S. V. Shiryaev, M. Baran, H. Szymczak, and R. Szymczak, Fiz. Nizk. Temp. 23, 159 ~1997! @Sov. J. Low Temp. Phys. 23, 116 ~1997!#; M. Baran, H. Szymczak, R. Szymczak, S. N. Barilo, V. I. Gatalskaya, and S. V. Shiryaev, J. Magn. Magn. Mater. 166, 124 ~1997!. 37 A. M. Campbell, J. E. Evetts, and D. Dew-Hughes, Philos. Mag. 18, 313 ~1968!. 38 W. A. Fietz and W. W. Webb, Phys. Rev. 178, 969 ~1969!. 39 A. M. Campbell and J. E. Evetts, Adv. Phys. 21, 199 ~1972!. 40 D. Dew-Hughes, Philos. Mag. 30, 293 ~1974!. 41 E. D. Kramer, J. Appl. Phys. 44, 1360 ~1973!. 42 K. Kishio, Y. Nakayama, N. Notohira, T. Noda, T. Kobayashi, K. Kitazawa, K. Yamafuji, I. Tanaka, and H. Kojima, Supercond. Sci. Technol. 5, 569 ~1992!. 43 T. Kobayashi, T. Kimurea, J. Shimoyama, K. Kishio, K. Kitazawa, and K. Yamafuji, Physica C 254, 213 ~1995!. 44 J. M. Li, F. R. deBoer, L. W. Roeland, M. J. V. Menken, K. Kadowaki, A. A. Menovsky, J. J. M. Franse, and P. H. Kes, Physica C 169, 81 ~1990!. 45 H. Theuss and H. Kronmuller, Physica C 177, 253 ~1991!. 46 R. Wördenweber, K. Heinemann, G. V. S. Sastry, and H. C. Freyhardt, Cryogenics 29, 458 ~1990!. 47 L. Civale, M. W. McElfrech, A. D. Marwick, F. Holtzberg, C. Felid, J. R. Thompson, and D. K. Christen, Phys. Rev. B 43, 13 732 ~1991!. 48 R. Hiergeist, R. Hergt, A. Erb, H. G. Schnack, and R. Grissen, Physica C 235–240, 2743 ~1994!. 49 M. Xu, D. K. Finnemore, K. Zhang, B. Dabrowski, G. W. Crabtree, and D. G. Hinks, in Proceedings of the Seventh International Workshop on Critical Currents in High Temperature Superconductivity, Alpbach, 1994, edited by H. W. Weber ~World Scientific, Singapore, 1994!, p. 323. 50 L. Klein, E. R. Yacoby, Y. Yeshurun, A. Erb, G. Muller-Vogt, V. Breit, and H. Wuhl, Phys. Rev. B 49, 4403 ~1994!. 51 H. Kumakura, K. Togano, N. Tomita, E. Yanagisawa, S. Okayasu, and Y. Kazumata, Physica C 251, 231 ~1995!. 52 R. Prozorov, A. Tsameret, Y. Yeshurun, G. Koren, M. Konczykowski, and S. Bouffard, Physica C 234, 311 ~1994!. 53 R. A. Rose, S. B. Ota, P. A. J. de Grovt, and B. Jayaram, Physica C 170, 51 ~1990!. PRB 58 54 SCALING OF MAGNETIZATION AND SOME BASIC . . . J. Y. Yuang, S. J. Wang, T. M. Uen, and Y. S. Gou, Phys. Rev. B 46, 1188 ~1992!. 55 L. Niel, Cryogenics 321, 975 ~1992!. 56 S. N. Barilo, D. I. Zhigunov, L. A. Kurochkin, A. V. Pushkarev, and S. V. Shiryaev, Sverkhprovodimost: Fiz. Khim. Tekh. 5, 1084 ~1992! @Sov. Phys. Supercond. 5, 1081 ~1992!. 57 S. N. Barilo, N. M. Olekhnovich, N. S. Orlova, A. V. Pushkarev, A. N. Salak, and S. V. Shiryaev, Cryst. Res. Technol. 31, 107 ~1996!. 58 R. R. Hake, Phys. Rev. 166, 471 ~1968!. 59 L. F. Mattheiss and D. R. Hamann, Phys. Rev. Lett. 60, 2681 ~1988!. 60 12 367 A. K. Gandopadhyay and J. S. Schilling, Physica C 264, 281 ~1996!. 61 Tablitsy Fizitheskikh Velithin, edited by I. K. Kikoin ~Atomizdat, Moscow, 1976!, p. 302. 62 A. M. Toxen, Phys. Rev. Lett. 15, 462 ~1965!. 63 M. Dauemling, J. M. Seunjens, and D. Larbalestver, Nature ~London! 346, 332 ~1990!. 64 N. Chikumoto, M. Konczykowski, N. Notohira, and A. P. Malozemoff, Phys. Rev. Lett. 69, 1260 ~1992!. 65 P. N. Kes and J. Van den Berg, in Studies of High Temperature Superconductors, edited by A. V. Narlikar ~Nova Science, New York, 1990!, Vol. 5, p. 83. 66 Y. Idemoto, Y. Iwata, and K. Fueki, Physica C 222, 257 ~1994!.